Active Standard ASTM E561 | Developed by Subcommittee: E08.07
Book of Standards Volume: 03.01
Historical (view previous versions of standard)
Significance and Use
5.1 The K-R curve characterizes the resistance to fracture of materials during slow, stable crack extension and results from the growth of the plastic zone ahead of the crack as it extends from a fatigue precrack or sharp notch. It provides a record of the toughness development as a crack is driven stably under increasing applied stress intensity factor K. For a given material, K-R curves are dependent upon specimen thickness, temperature, and strain rate. The amount of valid K-R data generated in the test depends on the specimen type, size, method of loading, and, to a lesser extent, testing machine characteristics.
5.2 For an untested geometry, the K-R curve can be matched with the crack driving (applied K) curves to estimate the degree of stable crack extension and the conditions necessary to cause unstable crack propagation (1).4 In making this estimate, K-R curves are regarded as being independent of original crack size ao and the specimen configuration in which they are developed. For a given material, material thickness, and test temperature, K-R curves appear to be a function of only the effective crack extension Δa e (2).
5.2.1 To predict crack behavior and instability in a component, a family of crack driving curves is generated by calculating K as a function of crack size for the component using a series of force, displacement, or combined loading conditions. The K-R curve may be superimposed on the family of crack driving curves as shown in Fig. 1, with the origin of the K-R curve coinciding with the assumed original crack size ao. The intersection of the crack driving curves with the K-R curve shows the expected effective stable crack extension for each loading condition. The crack driving curve that develops tangency with the K-R curve defines the critical loading condition that will cause the onset of unstable fracture under the loading conditions used to develop the crack driving curves.
5.2.2 Conversely, the K-R curve can be shifted left or right in Fig. 1 to bring it into tangency with a crack driving curve to determine the original crack size that would cause crack instability under that loading condition.
5.3 If the K-gradient (slope of the crack driving curve) of the specimen chosen to develop the K-R curve has negative characteristics (see Note 1), as in a displacement-controlled test condition, it may be possible to drive the crack until a maximum or plateau toughness level is reached (3, 4, 5). When a specimen with positive K-gradient characteristics (see Note 2) is used, the extent of the K-R curve which can be developed is terminated when the crack becomes unstable.
1.1 This test method covers the determination of the resistance to fracture of metallic materials under Mode I loading at static rates using either of the following notched and precracked specimens: the middle-cracked tension M(T) specimen or the compact tension C(T) specimen. A K-R curve is a continuous record of toughness development (resistance to crack extension) in terms of K R plotted against crack extension in the specimen as a crack is driven under an increasing stress intensity factor, K.
1.2 Materials that can be tested for K-R curve development are not limited by strength, thickness, or toughness, so long as specimens are of sufficient size to remain predominantly elastic to the effective crack extension value of interest.
1.5 The test is applicable to conditions where a material exhibits slow, stable crack extension under increasing crack driving force, which may exist in relatively tough materials under plane stress crack tip conditions.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
E4 Practices for Force Verification of Testing Machines
E399 Test Method for Linear-Elastic Plane-Strain Fracture Toughness K Ic of Metallic Materials
E1823 Terminology Relating to Fatigue and Fracture Testing
Other DocumentAISC Steel Construction Manual Available from American Institute of Steel Construction (AISC), One E. Wacker Dr., Suite 3100, Chicago, IL 60601-2001.
ICS Number Code 77.040.10 (Mechanical testing of metals)